advertisement

Eng. & Tech. Journal, Vol.28, No.6, 2010 Shear Capacity of High-Strength Fiber Reinforced Concrete Beam-Column Joints Dr. Kaiss Sarsam* & Zaid Muhammad Kani Al-Azzawi** Received on:2/9/2009 Accepted on:5/11/2009 Abstract This work examines the work of 13 high-strength concrete (HSC) beamcolumn joints (BCJ)-with and without steel fibers. Several shear design methods (with modification for fiber content, where applicable) were found to be conservative within a range of the following variables: 1) concrete compressive strength, 2) type and volume fraction of steel fibers, 3) content of hoops in the joint, and 4) column axial load. The coefficient of variation (COV) of the ratio of test strength to design strength (VTEST / VrDES) was found to be appreciably low for two of the five existing safe design methods. A conservative design method, which lowers the COV even further to a value of 7.8 percent, is proposed for HSC joints, with and without steel fiber reinforcement. Keywords:. Beam-column joints; Fiber reinforcement; High-strength concrete; Hoops; Shear strength. ﺍﻟﺘﺤﻤل ﺒﺎﻟﻘﺹ ﻟﻠﻤﻔﺎﺼل ﺒﻴﻥ ﺍﻷﻋﻤﺩﺓ ﻭﺍﻟﻌﺘﺒﺎﺕ ﺍﻟﻤﺼﻨﻭﻋﺔ ﻤﻥ ﺨﺭﺴﺎﻨﺔ ﻋﺎﻟﻴﺔ ﺍﻟﻤﻘﺎﻭﻤﺔ ﻭﺍﻟﻤﺴﻠﺤﺔ ﺒﺎﻷﻟﻴﺎﻑ ﺍﻟﺨﻼﺼﺔ ﻤﻔﺼل ﺒﻴﻥ ﺍﻟﻌﻤﻭﺩ ﻭﺍﻟﻌﺘﺒﺔ ﻤﺼﻨﻭﻋﺔ ﻤﻥ ﺨﺭﺴـﺎﻨﺔ ﻋﺎﻟﻴـﺔ13 ﻴﺸﻤل ﺍﻟﺒﺤﺙ ﻨﺘﺎﺌﺞ ﺍﺨﺘﺒﺎﺭ ﻴﺒﻴﻥ ﺍﻟﺒﺤﺙ ﺒﺄﻥ ﺘﻁﺒﻴﻕ. ﻤﻊ ﺃﻭ ﺒﺩﻭﻥ ﺍﻷﻟﻴﺎﻑ ﺍﻟﺤﺩﻴﺩﻴﺔ-ﺍﻟﻤﻘﺎﻭﻤﺔ ﻭﺍﻟﺘﻲ ﻓﺸﻠﺕ ﺒﺎﻟﻘﺹ ﻓﻲ ﺍﻟﻤﻔﺼل ﻭﺫﻟﻙ ﺒﻌﺩ ﺇﻀﺎﻓﺔ ﺘﻌﺩﻴل ﻋﻠﻴﻬﺎ،ﻋﺩﺓ ﻁﺭﻕ ﻤﺘﻭﻓﺭﺓ ﺤﺎﻟﻴﺎﹰ ﻟﻠﺘﺼﻤﻴﻡ ﻴﺅﺩﻱ ﺇﻟﻰ ﺘﺼﺎﻤﻴﻡ ﺃﻤﻴﻨﺔ ﻟﻠﻤﻔﺎﺼل ﻨﻭﻉ ﻭﻜﻤﻴﺔ، ﻤﻘﺎﻭﻤﺔ ﺍﻟﺨﺭﺴﺎﻨﺔ ﻟﻺﻨﻀﻐﺎﻁ: ﺘﺸﻤل ﻫﺫﻩ ﺍﻟﻨﺘﺎﺌﺞ ﻤﺘﻐﻴﺭﺍﺕ ﺃﺴﺎﺴﻴﺔ.ﻋﻨﺩ ﻭﺠﻭﺩ ﺍﻷﻟﻴﺎﻑ . ﻜﻤﻴﺔ ﺍﻷﻁﻭﺍﻕ ﻓﻲ ﺍﻟﻤﻔﺼل ﻭﻤﻘﺩﺍﺭ ﺍﻟﺤﻤل ﺍﻟﻤﺤﻭﺭﻱ ﻟﻠﻌﻤﻭﺩ،ﺍﻷﻟﻴﺎﻑ ﺍﻟﺤﺩﻴﺩﻴﺔ ﻴﻅﻬﺭ ﺍﻟﺒﺤﺙ ﺒﺄﻥ ﻤﻌﺎﻤل ﺍﻟﺘﻐﺎﻴﺭ ﻟﻠﻨﺴﺒﺔ ﺒﻴﻥ ﺘﺤﻤل ﺍﻟﻤﻔﺼل ﻟﻠﻘﺹ ﺒﺎﻻﺨﺘﺒﺎﺭ ﺇﻟﻰ ﺍﻟﺘﺤﻤل ﺍﻟﻤﺼﻤﻡ ﻋﻠﻴﻪ ﺃﻗل ﺒﻜﺜﻴﺭ ﻓﻲ ﺇﺜﻨﻴﻥ ﻤﻥ ﻁﺭﻕ ﺍﻟﺘﺼﻤﻴﻡ ﺍﻷﻤﻴﻨﺔ ﺍﻟﻤﺘﻭﻓﺭﺓ ﺤﺎﻟﻴﺎﹰ ﻤﻘﺎﺭﻨﺔ ﺒﺎﻟﻁﺭﻕ ﺍﻟﺜﻼﺜﺔ ﺍﻷﺨﺭﻯ ﻴﻘﺩﻡ ﺍﻟﺒﺤﺙ ﻁﺭﻴﻘﺔ ﺃﻤﻴﻨﺔ ﻤﻘﺘﺭﺤﺔ ﻟﺘﺼﻤﻴﻡ ﺍﻟﻤﻔﺎﺼل ﺍﻟﻤﺼﻨﻭﻋﺔ ﻤـﻥ ﺍﻟﺨﺭﺴـﺎﻨﺔ ﻋﺎﻟﻴـﺔ.ﺍﻷﻤﻴﻨﺔ ﺘﺅﺩﻱ ﺍﻟﻁﺭﻴﻘﺔ ﺍﻟﻤﻘﺘﺭﺤـﺔ ﺇﻟـﻰ. ﺇﺤﺘﻭﺍﺌﻬﺎ ﻋﻠﻰ ﺍﻷﻟﻴﺎﻑ ﺍﻟﺤﺩﻴﺩﻴﺔ ﺃﻭ ﺒﺩﻭﻨﻬﺎ:ﺍﻟﻤﻘﺎﻭﻤﺔ ﻓﻲ ﺍﻟﺤﺎﻟﺘﻴﻥ .% 7.8 ﻗﻴﻤﺘﻪ،ﻤﻌﺎﻤل ﺘﻐﺎﻴﺭ ﺃﻗل Introduction The use of high-strength concrete (HSC) in construction has steadily increased over the past years leading to the reduction of member sizes. Several studies have demonstrated the economy of using HSC in low-rise, mid-rise and high- rise buildings(1). The increasing use of HSC has raised the concern over the applicability of the current empirical methods, which were developed from experimental data on specimens having compressive strength below 40 MPa(1). * Building & Construction Engineering Department, University of Technology/ Baghdad. ** College of Engineering, University of Anbar/ Anbar 1253 PDF created with pdfFactory Pro trial version www.pdffactory.com Eng. & Tech. Journal. Vol.28, No.6, 2010 Shear Capacity of High-Strength Fiber Reinforced Concrete BeamColumn Joints and possible voids within the joint core. Test results(13-15) have shown that the shear capacity and ductility of the BCJ region is increased when steel fiber reinforced concrete (SFRC) is used. Thus, the hoop reinforcement in the joint may be reduced or eliminated by using SFRC in the BCJ region. Research Significance HSC joint tests with and without fibers are compared with several simple design methods, including code design originally developed mainly from NSC research. All existing design methods [Eqs. (2-7)] are identical to their respective requirement for shear design, except for the addition of a term for steel fiber contribution, where applicable. A proposed method is introduced that leads to a conservative design. Experimental Program Full details of test specimens and material properties are available in reference 17. Table 1 and Fig. 1 give specimen details. All reinforcing bars were deformed, except the 4mm hoop bars (Table 1) which were plain. Yield strengths of the 4-, 8-, 12-, 16-, and 18-mm bars were 557, 466, 440, 507, and 531 MPa, respectively. Mix proportions by weight of 1:1.24:1.86:0.285:0.05 were used respectively for the cement, sand, gravel, water, and superplasticizer. Steel fibers of 1100 MPa tensile strength were used. The straight fibers had a length of 25.4mm, a diameter of 0.4mm and an aspect ratio (L/D) of 63.5; while the hooked fibers had a length of 50mm, a diameter of 0.5mm and an aspect ratio of 100. HSC, as a material in compression may be brittle, and as the concrete strength increases the post peak portion of the stress-strain diagram almost vanishes or descends steeply(2-6). The decrease in ductility could be a serious drawback for HSC. Research indicates that steel fibers are more effective in increasing both strength and ductility of HSC than those of normal-strength concrete (NSC)(7) . This is due to the improved bond characteristics associated with the use of fibers in HSC as compared to NSC. The use of fibers to improve the characteristics of construction materials is well established(8-11) . The addition of fibers transforms concrete into a more ductile material. The randomly oriented fibers arrest the concrete microcracking mechanism and limit crack propagation, thus improving strength and ductility. The beam-column joint (BCJ) is one of the most critical areas of a framed structure, where failure is often initiated because of high shearing forces. The increasing use of HSC in columns(1) made the HSC joint design of paramount importance in the design of framed buildings. To dissipate the energy introduced by the loading, the BCJ region should be designed with sufficient strength and ductility to allow a plastic hinge to develop in the beam rather than in the column. A BCJ is currently designed to withstand a large shearing forces by closer spacing of joint hoops(12). However the spacing reduction may prevent concrete from flowing around the reinforcing bars during construction, causing inadequate bond between the steel and concrete 1254 PDF created with pdfFactory Pro trial version www.pdffactory.com Eng. & Tech. Journal. Vol.28, No.6, 2010 Shear Capacity of High-Strength Fiber Reinforced Concrete BeamColumn Joints This indicates that repair after damage (retrofitting) could be easier if the BCJ with fibers is used. The expected influence of the column axial load in increasing the joint diagonal cracking angle with the horizontal can be clearly seen by comparing the failure of SP-3 [Fig. 2(b)] and SP-13 [Fig. 2(f)]. The cracks in the latter with a column compressive stress of 6.41 MPa were more vertical in the joint as compared with the former that has a column compression stress of 3.21 MPa. The behavior of each of the 13 BCJs indicates no anchorage distress in the beam and column reinforcement at failure. The BCJ failure load capacity (VTEST of Table 1) is based on equilibrium at the column-beam interface. The exerted external moment at failure (Mmax in the beam) is equated to the internal resisting moment of the beam crosssection at the beam-column interface. Then the forces (tension and compression) are added algebraically to obtain a net zero axial force in the interface. The contribution of the fibers is included in the tension zone of the cross-section. Detailed calculations of VTEST are presented in reference 17. Evaluation Of Experimental Results Joint strength design equations: Regression analysis of the results of the 13 BCJ tests of this work under monotonic loading has resulted in the proposed Eq. (1). As will be seen later, Eq. (1) leads to an improved conservative strength prediction of HSC joints, with and without fiber. In all of the following [Eqs. (1-7)] the symbols are defined Special bearing assemblies (rollers and hinges) were made to facilitate the application of the loads to the test specimens in the testing rig. The column was loaded to a prespecified compression load Nu prior to any beam loading. This axial load was kept constant in each BCJ test. Experimental Results All of the 13 BCJs failed in joint shear. Fig. 2 shows the joint failure of specimens SP-1, SP-3, SP-8, SP-9, SP-10, and SP-13. Firstly, the beam flexure tension cracks started in a similar way for all 13 specimens, near the beam-joint interface and expanded into the beam. Secondly, the joint diagonal cracks appeared, for all specimens, nearly parallel to the joint diagonal. For BCJs without fibers, there was a central dominant crack with a few additional cracks to its side (e.g. specimens SP-1 & SP-8) as shown in Figs. 2(a) and 2(c). However, the crack patterns were significantly different from those in BCJs with fibers with several more cracks. The crack size in BCJ's with fibers was much smaller than that on BCJs without fibers (e.g. specimens SP-3 &SP-10) as shown in Figs. 2(b) and 2(e). The existence of a hoop did not prevent a brittle type failure, as can be seen when comparing SP-8 failure [Fig. 2(c)] which had no fibers with SP-9 [Fig. 2(d)] which was identical except for 1.0% hooked fibers (each had a single 8mm central hoop in the joint). The latter had a greater number of smaller size cracks at failure than the former. In addition, the integrity at failure of SP-9 was significantly better than that of SP-8. 1255 PDF created with pdfFactory Pro trial version www.pdffactory.com Eng. & Tech. Journal. Vol.28, No.6, 2010 Shear Capacity of High-Strength Fiber Reinforced Concrete BeamColumn Joints in the "Notation" except where necessary [e.g. Eqs. (1-A), (1-B), etc.]. VrPROP = [ 1 + 0.29 N VrC 352 = 0.85 [1.4 × 0.29 f c′ 1 + 0.29 u Ag Asv . f yv . d c b′ . d c + ] + VF ......... (3) Sv ] d f cf′ + 10 F + 24 ρ d . c . db Modified Meinheit's method(16) 2/3 VrMEIN = Vc + Vs = 0.97 [ξ . ( fc′ ) . bc . d c ] + VF …........... (4) where: ... (4-A) ξ = 1 + 6 ρ s ≤ 1.6 A (2b ′ + 2h ′) ... (4-B) ρs = h Sv . b′ . h′ and ... (4-C) VrMEIN ≤ 1.66 f c′ . bc . d c Nu 1 . bc . d c + . Ast . f yv Ag β …... (1) where F = Vf . L .d f D ….. (1-A) The fiber influence (VF) is defined as follows: d N VF = (10F ). c . 1 + 0.29 u . bc . d c Ag db Modified British Standard method(20) ….. (1-B) 1/ 3 fcf′ is substituted into the value of fc′ where applicable. The design methods modified with Eq. (1-B) are defined as follows: Modified ACI code method(21) f c′ N VrACI = 0.85 [ . 1 + u . bc . d c 6 14 Ag Asv . f yv . d c + ] + VF ………….... (6) Sv Modified Sarsam's method(18) dc db 1/ 3 VrSARS = [5.43( f c′ . ρ c ) . 1/ 4 100 As 400 . . VrBS = [0.79 bc . d c d c 0.87 Asv . f yv . d c 1 ] + VF bc . d c + 1.25 Sv …... (5) Because the following methods [Eqs. (2) to (6)] do not include the influence of the fiber fraction, an additional term is added [Eq.(1-B)]. In Eqs. (2) to (6), the value of . 4/3 . Modified Beckingsale's method(22) f ′ Nu VrBECK = 0.85 [0.25 1 + c . − 2.5 . 25 Ag N 1 + 0.29 u . bc . d c + 0.87 Ast . f yv ] + VF Ag …... (2) bc . hc + Ast . f yv ] + VF Modified ACI-ASCE COMM.352 method(19) ………... (7) Comparison of design methods: Table 2 compares the seven design methods for all HSC 1256 PDF created with pdfFactory Pro trial version www.pdffactory.com Eng. & Tech. Journal. Vol.28, No.6, 2010 Shear Capacity of High-Strength Fiber Reinforced Concrete BeamColumn Joints specimens. Considering a ratio of VTEST / VrDES ≥ 1.0 as conservative, all design equations except Eq. (4) lead to a safe design. The percent coefficient of variation (COV) corresponding to Eqs. (7, 6, 5, 3, 2 and 1) are: 54.8, 37.6, 35.1, 16.1, 11.0 and 7.8, respectively. Influence of major parameters The prediction accuracy of the three conservative design methods with the lowest COV percentage is compared in Figs. 3 through 6. Fig. 3 shows the influence of the fiber factor (F) on the safety of prediction (ratio of VTEST / VrDES). It can be seen that the predictions of the modified methods of Sarasm [Eq. (2)] and Committee 352 [Eq. (3)] indicates significant drops in their safety margins with increasing F values. In contrast, the proposed Eq. (1) does not show any significant change in safety with rising F values. Similarly, Fig.4 indicates that both Eqs. (2) and (3) lead to significant drops in safety factor with rising fcf′ 1- 2- 3- 4- values, in contrast with the proposed Eq. (1). Fig. 5 shows that the three design methods show no significant change in the safety factor with the hoop force value ( Ast . f yv ). However, 5- the proposed Eq. (1) shows little scatter in the predictions compared to those predicted by Eqs. (2) and (3). Similarly Fig. 6 shows that predictions obtained using Eqs. (2) and (3) are scattered in contrast to those obtained when using the proposed Eq. (1). Conclusions Based on the thirteen HSC joint tests, the following conclusions can be made: 6- HSC joints without fibers exhibited sudden modes of failure, even for specimens with hoops that fractured. Therefore, it is not recommended to construct HSC joints without fibers unless the designer ensures that the failure would be outside the joint by considering all the design variables including overstrength of the adjoining members(23). The addition of fibers in the BCJs helped to keep significantly better integrity of specimens at failure load, in contrast with joints without fibers. The observed large number of smaller size cracks for specimens with steel fibers have led to more ductile behavior as compared to BCJs without fibers. Table 1 shows that there may be an upper limit to the usefulness of Vf for both straight and hooked fibers. Using 0.5% and 1.0% for Vf succeeded in strengthening the joint. In contrast, using 1.5% for Vf led to a drop in strength compared to BCJs with 1.0% for Vf . All 13 HSC joints could be safely designed using 6 of the 7 methods. The exception is reference 16, which leads to 12 unsafe strength predictions. The severe loading (reversible cyclic) regime of testing in New Zealand(22) has led to exceedingly conservative design requirements. For example the mean of the shear design values obtained by using Eq. (7) (Table 2) is 3.8 times that of the mean of the shear design values obtained by using Eq. (1). 1257 PDF created with pdfFactory Pro trial version www.pdffactory.com Eng. & Tech. Journal. Vol.28, No.6, 2010 Shear Capacity of High-Strength Fiber Reinforced Concrete BeamColumn Joints Both BS(20) and ACI(21) design methods, which are essentially based on beam (rather than BCJ) shear tests, give rather high COV values of 35.1% and 37.6% respectively. 8- The proposed method [Eq. (1)] gives the lowest COV among the three BCJ design methods- Eqs. (1-3). These COV values for HSC joints (with or without fibers) were 16.1%, 11.0% and 7.8% for Eqs. (3), (2) and (1) respectively. 9- Based on this work, using steel fibers for HSC joints with an upper limit of 1.0% volume fraction has proved to be successful in improving both the ductility and strength of BCJs. This applies to joints with and without hoops. 10- Current existing design methods, except reference 16, were found to be conservative for HSC joint design, with and without fibers. Further Research Further research is indicated in the following: 1- Influence of a large amount of hoop reinforcement in HSC joint. 2- Influence of different beam-tocolumn relative dimensions. 3- Behavior of ultra high-strength concrete (UHSC) jointsexceeding 100 MPa in compressive strength. 4- Influence of very high column compression load on BCJ behavior. 5- Influence of column tensile load on BCJ behavior. 6- Influence of reversible cyclic loading on fiber reinforced HSC joint behavior. 7- Influence of prestressing on fiber reinforced BCJ behavior. Acknowledgment This work was sponsored by Al-Rasheed Contracting Company and the Building and Construction Engineering Department, University of Technology, Baghdad, Iraq. The authors express their gratitude to all who helped, including the staff of the Directorate of Productive Factories and Structures Laboratory. Notations 7- Ag Ah As Asc Aso Ast Asv b' bc D db dc df F = gross cross-section area of the column at the joint. = cross-sectional area of one leg of a hoop. = area of tensile reinforcement. = area of two layers of column longitudinal reinforcement at two opposite faces- i.e. not including intermediate bars. = area of the layer of column longitudinal reinforcement furthest away from the maximum column compression face. = total area of hoops crossing the diagonal plane from corner to corner of the joint between the beam compression and tension reinforcement = cross-sectional area of one layer of hoops perpendicular to the member longitudinal reinforcement. = external width of hoops. = width of column section at the joint. = fiber diameter. = distance from extreme beam compression fiber to centroid of tension reinforcement. = distance from extreme column compression face to centroid of the layer of column steel furthest away from this face. = fiber bond factor, = 0.5 for hooked fibers, = 0.25 for straight fibers. = fiber factor- Eq. (1-A). 1258 PDF created with pdfFactory Pro trial version www.pdffactory.com Eng. & Tech. Journal. Vol.28, No.6, 2010 f c′ fcf′ fyv h' hc L Nu Sv Vc VF Vf VrACI VrBECK VrBS VrC352 vrDES VrMEIN VrPROP VrSARS Vs VTEST β ρc ρd Shear Capacity of High-Strength Fiber Reinforced Concrete BeamColumn Joints = concrete compression strength based on 150 x 300 mm cylinders. = fiber reinforced concrete compression strength based on 150 x 300 mm cylinders. = yield strength of hoops. = external depth of hoops. = total depth of column. = fiber length. = column axial load. = spacing of hoops. = shear force resistance of hoops. = shear force resistance of fibersEq. (1-B). = fiber volume fraction. = design joint shear resistance by Eq. (6)*. = design joint shear resistance by Eq. (7)*. = design joint shear resistance by Eq. (5)*. = design joint shear resistance by Eq. (3)*. = design joint shear resistance*. = design joint shear resistance by Eq. (4)*. = design joint shear resistance by Eq. (1)*. = design joint shear resistance by Eq. (2)*. = shear force resistance of hoops. = BCJ failure load capacity. = constant factor, = 1.0 with one layer of hoops in the middle of the joint, = 1.5 with more than one layer of joint hoops. = Aso /(bc . dc ). = Asc /(bc . hc ). V. 81, No. 4, July-August 1984, pp. 364-411. [3]-Swamy, R. N. , "HighStrength Concrete- Material Properties and Structural Behavior", High-Strength Concrete, ACI Publication, SP87, 1985, pp. 119-146. [4]-Carrasquillo, R. L. ; Nilson, A. H. ; and Slate, F. O. , "Properties of High-Strength Concrete Subjected to Short Term Loads", ACI Journal, V.78, No. 3, May-June 1981, pp. 171178. [5]-Martines, S. ; Nilson A. H. ; and Slate, F. O. , "Spirally Reinforced High-Strength Concrete columns", ACI Journal, V. 81, No. 5, Sep.- Oct. 1984, pp. 431-442. [6]-Slate, F. O. ; Nilson A. H. ; and Martines, S. , "Mechanical Properties of High-Strength Lightweight Concrete", ACI Journal, V. 83, No. 4, July-Aug. 1986, pp. 606-613. [7]-Valle, M. ; and Büyüköztürk, O. , "Behavior of Fiber Reinforced High-Strength Concrete under Direct Shear", ACI Materials Journal, V. 90, No. 2, Mar.- Apr. 1993, pp. 122133. [8]-ACI Committee 544, "Stateof- the Art Report on Fiber Reinforced Concrete", ACI Manual of Concrete Practice, 1990. [9]-Romualdi, J. P. ; and Baston, G. B. , "Mechanics of Crack Arrest in Concrete", Journal of the Engineering Mechanics Division, ASCE, V. 89, No. EM5, June 1963, pp. 147-168. * All Vr values include the appropriate material reduction factors. References [1]-ACI-ASCE Committee 441, "High-Strength Concrete Columns: State of the Art", ACI 441R-96, ACI Structural Journal, V. 94, No. 3, May-June 1997, pp. 323-335. [2]-ACI Committee 363, "State Of the Art Report on HighStrength Concrete", ACI Journal, 1259 PDF created with pdfFactory Pro trial version www.pdffactory.com Eng. & Tech. Journal. Vol.28, No.6, 2010 Shear Capacity of High-Strength Fiber Reinforced Concrete BeamColumn Joints Joints", MSc Thesis, Building and Construction Engineering Department, University of Technology, Baghdad, Iraq, Dec. 1997, 178 PP. [18]-Sarsam, K. F. , "Strength and Deformation of Structural Concrete Joints", PhD Thesis, The University of Manchester Institute of Science and Technology, Manchester (U.K.), 1983, 340 PP. [19]-ACI-ASCE Committee 352, "Recommendations for Design of Beam-Column Joints in Monolithic Reinforced Concrete Structures", ACI Journal, V. 73, No. 7, July 1976, pp. 375-393. [20]-British Standards Institution, "Structural Use of Concrete", BS 8110: 1985, Parts 1and 2. [21]-ACI Committee 318, "Building Code Requirements for Structural Concrete (ACI 318M- 99 / ACI 318 RM- 99)", American Concrete Institute, 1999, 391 PP. [22]-Beckingsale, C. W. , " PostElastic Behavior of Reinforced Concrete Beam-Column Joints", PhD Thesis, Department of Civil Engineering, University of Canterbury, New Zealand, Aug. 1980, 359 PP. [23]-Bresler, B. ; and Bertero, V. V. , "Olive View Medical Center- Materials Studies, Phase I", Report No. EERC 73-19, University of California, Berkeley, 1973. [10]-Naaman, A. E. , "Fiber Reinforcement for Concrete", Concrete International: Design & Construction, V. 7, No. 3, March 1985, pp. 21-25. [11]-Naaman, A. E. ; and Homrich, J. R. , "Properties of High-Strength Fiber Reinforced Concrete", ACI Publication, SP87, 1985, pp. 233-249. [12]-ACI-ASCE Committee, "Recommendations for Design of Beam-Column Joints in Monolithic Reinforced Concrete Structures", ACI Journal, V. 82, No. 3, May-June 1985, pp. 266283. [13]-Henager, C. H. , "Steel Fibrous, Ductile Concrete Joints for Seismic-Resistant Structures", Reinforced Concrete Structures in Seismic Zones, ACI Publication, SP-53, 1977, pp. 371-386. [14]-Jindal, R. L. ; and Hassan, K. A. , "Behavior of Steel Fiber Reinforced Concrete BeamColumn Connections", Fiber Reinforced Concrete, ACI Publication, SP-81, 1984,pp. 107-123. [15]-Craig, R. J. ; and Mahadev, S. ; Patel, C. C. ; Viteri, M. ; and Kertesz, C. , "Behavior of Joints Using Reinforced Fibrous Concrete", ACI Publication, SP81, 1984, pp.125-167. [16]-Meinheit, D. F. ; and Jirsa, J. O. , "Shear Strength of R/C Beam-Column Connections", Journal of Structural Division, ASCE, V. 107, No. ST-11, Nov. 1981, pp. 2227-2244. [17]-Al-Azzawi, Zaid M. K. , " Capacity of High-Strength FiberReinforced Beam-Column 1260 PDF created with pdfFactory Pro trial version www.pdffactory.com Eng. & Tech. Journal. Vol.28, No.6, 2010 Shear Capacity of High-Strength Fiber Reinforced Concrete BeamColumn Joints Table(1) Test details and results 1261 PDF created with pdfFactory Pro trial version www.pdffactory.com Eng. & Tech. Journal. Vol.28, No.6, 2010 Shear Capacity of High-Strength Fiber Reinforced Concrete BeamColumn Joints Table (2) Comparison between νTEST and νrDES 1262 PDF created with pdfFactory Pro trial version www.pdffactory.com Eng. & Tech. Journal. Vol.28, No.6, 2010 Shear Capacity of High-Strength Fiber Reinforced Concrete BeamColumn Joints Figure (1) Specimen details 1263 PDF created with pdfFactory Pro trial version www.pdffactory.com Eng. & Tech. Journal. Vol.28, No.6, 2010 Shear Capacity of High-Strength Fiber Reinforced Concrete BeamColumn Joints Figure (2) Specimens after failure 1264 PDF created with pdfFactory Pro trial version www.pdffactory.com Eng. & Tech. Journal. Vol.28, No.6, 2010 Shear Capacity of High-Strength Fiber Reinforced Concrete BeamColumn Joints 1265 PDF created with pdfFactory Pro trial version www.pdffactory.com Eng. & Tech. Journal. Vol.28, No.6, 2010 Shear Capacity of High-Strength Fiber Reinforced Concrete BeamColumn Joints 1266 PDF created with pdfFactory Pro trial version www.pdffactory.com